Open access

# Polymer Nanocomposite Hydrogels for Water Purification

Written By

Manja Kurecic and Majda Sfiligoj Smole

Submitted: February 29th, 2012 Published: September 27th, 2012

DOI: 10.5772/51055

From the Edited Volume

## Nanocomposites

Chapter metrics overview

View Full Metrics

## 1. Introduction

Contamination of water, due to the discharge of untreated or partially treated industrial wastewaters into the ecosystem, has become a common problem for many countries [1]. In various productions, such as textiles, leather, rubber, paper, plastic and other industries, the dyeing processes are among the most polluting industrial processes because they produce enormous amounts of coloured wastewaters [2-4]. In addition to their colour, some of these dyes may degrade to highly toxic products, potentially carcinogenic, mutagenic and allergenic for exposed organisms even at low concentrations (less than 1 ppm) [5]. They contaminate not only the environment but also traverse through the entire food chain, leading to biomagnifications [6-9]. The removals of such compounds particularly at low concentrations are a difficult problem.

Textile effluents are usually treated by physical and chemical processes such as sorption, oxidation, flocculation, etc. Colour removal by activated carbon, H2O2, sodium hyperchlorite and other chemical agents has been widely practiced in the textile industries [10]. Although activated carbon remains the most widely used adsorbent, its relatively high cost restricts its use sometimes. However, in addition to, adsorptive properties and availability are also key criteria when choosing an adsorbent for pollutant removal, thereby encouraging research into materials that are both efficient and cheap. Many non-conventional low-cost adsorbents, including natural materials, biosorbents, and waste materials from agriculture and industry have been proposed by several researchers [11-14]. Considering low cost, abundance, high sorption properties and potential ion-exchange, clay minerals are interesting materials for use as adsorbents, since they can be easily obtained and regenerated [7].

## 2. Clay minerals

Clays are widely applied in many fields such as polymer nano-composites [15-18], catalysts [19,20], photochemical reaction fields [21], ceramics [22], paper filling and coating [23], sensors and biosensors [24], absorbents, etc. due to their high specific surface area, chemical and mechanical stabilities, and a variety of surface and structural properties [25].

The most-used clays are smectite group which refers to a family of non-metallic clays primarily composed of hydrated sodium calcium aluminium silicate, a group of monoclinic clay-like minerals with general formula of (Ca,Na,H)(Al,Mg,Fe,Zn)2(Si,Al)4O10(OH)2 nH2O.

Smectite is a clay mineral having a 2:1 expanding crystal lattice (Figure 1). Its isomorphous substitution gives various types of smectite and causes a net permanent charge balanced by cations in such a manner that water may move between the sheets of the crystal lattice, giving a reversible cation exchange and very plastic properties.

Members of the smectite group include the dioctahedral minerals montmorillonite, beidellite, nontronite, bentonite, and the trioctahedral minerals hectorite (Li-rich), saponite (Mg-rich) and sauconite (Zn-rich). The basic structural unit is a layer consisting of two inward-pointing tetrahedral sheets with a central alumina octahedral sheet. The layers are continuous in the length and width directions, but the bond between layers are weak and have excellent cleavage, allowing water and other molecules to enter between the layers causing expansion in the third direction [15,16,25,26].

In the inner blocks, all corners of silica tetrahedra are connected to adjacent blocks, but in outer blocks some of the corners contain Si atoms bound to hydroxyls (Si-OH). These silanol groups at the external surface of the silicate, are usually accessible to organic species, and act as neutral adsorption sites. In addition to, some isomorphic substitutions occur in the tetrahedral sheet of the lattice of the mineral form leading to negatively charged adsorption sites which are occupied by exchangeable cations [25]. These characteristic make them powerful absorbents for organic molecules and organic cations. In order to improve the adsorption properties of clay absorbents also for organic anions, clay surface can be modified. There are many exchangeable cations on the clay surface therefore the cationic surfactants are generally used as modifiers. The characteristics of these so-called organoclays can be changed by variation of surfactant properties, such as alkyl chain length, etc. The surface properties of the clays modified by surfactants alter from organophobic to organophilic, which aids in improving clay adsorption capacities for organic compounds [27]. While crude clay minerals are effective for the adsorption of cations, organo-modified clays may adsorb negative and hydrophobic molecules [25]

### 2.1. Organically modified clay minerals

Surface modifications of clay minerals have received great attention because it allows the creation of new materials and new applications [28]. Organically modified clay minerals have become essential for development of polymer nanocomposites. Modified clays are also used in other applications such as adsorbents of organic pollutants in soil, water and air; rheological control agents; paints; cosmetics; refractory varnish; thixotropic fluids, etc. Several routes can be employed to modify clays and clay minerals [29]:

• ion exchange with inorganic cations and organic cations,

• binding of inorganic and organic anions (mainly at the edges),

• grafting of organic compounds, reaction with acids,

• pillaring by different types of poly(hydroxo metal) cations,

• intraparticle and interparticle polymerization,

• dehydroxylation and calcination,

• delamination and reaggregation of smectites,

• lyophilisation,

• ultrasound, and

• plasma.

Ion exchange with alkylammonium ions is well-known and the preferential method to prepare organoclays. Generally, the papers describe the preparation of the organoclays in laboratory scale, with different experimental conditions, clays from several regions and suppliers, and several kinds of organic compounds [28].

The research of intercalation of organic molecules into the interlayer space of clay minerals started in the 1920s, after the introduction of X-ray diffraction in 1913 [28]. Geseking [30] found methylene blue to be very effective in replacing interlayer cations. These results indicated on the possibility of using ammonium ions of the NH3R+, NH2R2+, NHR3+, and NR4+ types for better understanding of the mechanism of cation exchange in clay minerals. Different types of clay minerals were treated with the solution of hydrochlorides or hydroiodides of various amines. The clay minerals adsorbed the organic ions and increased the basal spacing more than those of the same clay minerals saturated with smaller cations such as calcium or hydrogen.

In 1944 MacEwan observed that when montmorillonite was treated with glycerol, a very sharp and intense first-order x-ray diffraction reflexion was obtained, corresponding to the basal spacing of 1.77 nm. The increase of basal spacing was due to the intercalation of glycerol into the interlayer space of the clay mineral. [31].

Studies of interactions between clay minerals and organic compounds have been presented, among others, in [32-34]. Clay–organic complexes of great industrial importance are the organoclays prepared from smectites and quaternary ammonium salts.

### 2.2. Organically modified clay minerals for dye adsorption

There are more than 100 000 types of dyes commercially available, with over 7 x 105 tons of dyestuff produced annually, which can be classified according to their structure as anionic and cationic. In aqueous solution, anionic dyes carry a net negative charge due to the presence of sulphonate (SO3¯) groups, while cationic dyes carry a net positive charge due to the presence of protonated amine or sulphur containing groups. [35]

Reactive dyes are extensively used in the textile industry because of their wide variety of colour shades, brilliant colours, and minimal energy consumption [36]. Therefore, considerable amount of research on wastewater treatment has focused on the elimination of these dyes, essentially for three reasons: firstly, reactive dyes represent 20-30% of the total dye market; secondly, large fraction of reactive dyes (10-50%) are wasted during the dyeing process (up to 0,6 – 0,8 g dye/dm3 can be detected in dyestuff effluent); thirdly, conventional wastewater treatment methods, which rely on adsorption and aerobic biodegradation, were found to be inefficient for complete elimination of many reactive dyes. [35]

In several research articles it is indicated that clay derivatives are potentially very promising sorbents for environmental and purification purposes. Although the modification of clays with surfactants increases their cost significantly, the resultant increase in adsorption capacity may still made surfactant-modified clays cost effective. The nano-clay, montmorillonite, and some modified nano-clays were used as sorbents for non-ionic, anionic and cationic dyes [41]. From the sorption differences among the different dye and clay structures, both chemical and morphological, the sorption forces that played important roles were identified. Nano-clays frequently have a sorption capacity of more than 600 mg sorbate per gram of sorbent at a liquor-to-sorbent ration of 100:1. Furthermore, a sorption of 90% at the initial dye concentration of 6g/L, or 60% based on the weight of sorbent, was observed. This indicates an extremely high dye affinity. This study showed that by modification of the nano-clay MMT, it can easily become an excellent sorbent for anionic, cationic and non-ionic dyes.

Clay minerals are in most cases used as dispersed adsorbents and as such aggravate the removal of adsorbents from clean purified water. Recently, there have been some activities to incorporate clay particles into nanocomposite hydrogels for application in wastewater technologies [42-45]. Incorporation of clay minerals in hydrogel matrix allows better manipulation with adsorbing material since clay minerals are fixed in the matrix.

## 3. Clay/polymer nanocomposite hydrogels

Hydrogels are 3D dense cross linked polymer network structure, containing hydrophilic and hydrophobic parts in a defined proportion. When placed in aqueous medium, they intensively swell. By swelling they increase their initial volume for several times without either dissolving or considerably changing their shape, because hydrophilic chains contact one to the other by cross-linking [42,46,47]. The response of hydrogel is dependent on the presence of hydrophilic functional groups such as –OH, -COOH. These groups make the hydrogel hydrophilic and due to the capillary action and the difference in the osmotic pressure, water diffuses into the hydrogel.

Polymerization methods, the presence of functional groups and the nature of cross-linking agents are important parameters that control the swelling ability of hydrogel [43].

Owing to their advantageous properties, such as swellability in water, hydrophilicity, biocompatibility and lack of toxicity, hydrogels have been utilized in a wide range of hygienic, agricultural, medical and pharmaceutical applications and in such applications, water absorbency and water retention properties are essential [46,48]. The most well-established hydrogel applications are superasorbing hydrogels in diapers and hydrogels for contact-lenses, just to mention few [49-53].

Recently hydrogels have gain particular interest in wastewater treatment due to their high adsorption capacities, especially regeneration abilities and reuse for continuous processes [54]. But pure hydrogels often have some limitations such as low mechanical stability and gel strength. In the initial phase of nanocomposite hydrogels development, various clay minerals were widely added to polymer hydrogel matrix in order to improve weak mechanical stability of hydrogels. Sodium montmorillonite (NaMMT) or attapulgite were used as reinforcing filler in the preparation of hydrogels to improve mechanical properties or swelling ability (55-58). Liang et al. [59] used organically modified montmorillonite to prepare hydrogels that exhibited higher swelling degree and enhanced thermal response compared to conventional poly(N-isopropylacrylamide) (PNIPAM) hydrogels. Hydrogels were also prepared with ionic monomers and montmorillonite [60]. However, the transparency, swelling degree and mechanical property did not improve simultaneously, in particular at relatively high NaMMT loading, because of the poor dispersion of clay mineral particles and structural inhomogeneity of the hydrogel network caused by the crosslinker N,N-methylene-bis-acrylamide (BIS) [61]. To overcome this problem, a special type of an inorganic-organic thermo-responsive PNIPAM nanocomposite hydrogel was developed by Haraguchi, containing laponite XLG without any chemical crosslinker. The exfoliated laponite particles acted as multifunctional crosslinker, and the polymer chains were anchored to the particles and entangled to form a network [49,50,53]. According to this mechanism several researches prepared various nanocomposite hydrogels by using laponite as multifunctional crosslinker [56,61]. The resulting hydrogels exhibited not only excellent optical and ultrahigh mechanical properties but also large swelling ratios and rapid shrinking capability [49,50,53,61,62].

Despite of undesired low mechanical properties, which can be improved by introduction of clay minerals in the hydrogel matrix, hydrogels have many predominant properties including low interfacial tension and a variety of functional groups which can trap ionic dyes from wastewater and provide high adsorption capacities [63]. Introduction of clay materials into hydrogel combines improvement of elasticity and permeability of the hydrogels with high ability of the clays to adsorb different substances. Application of low-priced and biodegradable adsorbents is a good tool to minimize the environmental impact caused by dye manufacturing and textile effluents. Consequently, research concerning development of hydrogels with clay particles for adsorbing dyes and metal ions is exponentially increasing [43,42,54,64].

Shirsath et al. synthesized polymer nanocomposite hydrogels using metal hybrid polymer along with clay. Ultrasonic irradiation was used to initiate the emulsion polymerization to form hydrogel through the generation of free radicals. The high shear gradients generated by the acoustic cavitations process help to control the molecular weight of hydrogels formed in aqueous solutions. Ultrasound was found to be an effective method for polymerization of monomers and for the production of hydrogel in the absence of a chemical initiator [43].

### 3.1. Clay/polymer nanocomposite synthesis

Hydrogels are usually crosslinked during polymerization via condensation polymerization or free radical polymerization (thermal polymerization, radiation polymerization, photo-polymerization or plasma polymerization) [65-67]. Photo-polymerization, in addition to its environmental-friendly aspects, offers a number of advantages, such as ambient temperature operations, location and time-control of the polymerization process and minimal heat production, in comparison with other techniques [68]. Photo-polymerization can be induced by ultraviolet (100-400 nm), visible (400-700 nm) or infrared (780-20000 nm) radiation. Light quanta are absorbed by molecules via electronic excitation [66]. During photo-polymerization process, photo-initiators are generally used having high absorption capacities at specific wavelengths of light thus enabling them to produce radically initiated species [69].

The preparation of a clay mineral-polymer composite with light for initiation of polymerization requires suitable monomers and a suitable photoiniciating system. In the research PNIPAM/clay nanocomposite hydrogels were synthesized using aqueous dispersion of organo-clay (O-MMT) particles, modified by distearyldimethyl ammonium chloride (Nanofil 8, Süd Chemie, Germany) in varied concentrations (0, 0.25, 0.5, 0.75, 1 wt% regarding the monomer content). Aqueous dispersions of different concentration of O-MMT were kept under constant stirring for 2 hours at room temperature after the addition of 1% NIPAM and 1 wt% (regarding the monomer content) BIS. After this period, 1 wt% (regarding the monomer content) Irgacure 2959 photoiniciator was added and the dispersion was kept under the same conditions for additional 1 hour. Prepared dispersions were pored in glass Petri dishes, bubbled with nitrogen for 5 minutes and covered. Petri dishes were placed on the sample holder in the middle of a UV chamber (Luzchem). Polymerization was carried out in UV chamber using 6 UVA lamps (centred at 350 nm) placed on top of the chamber with the distance to the sample 15 cm. Time of polymerization was 2 hours. After polymerization the hydrogels were washed with deionised water for 4 days (daily exchange of water). After washing, the hydrogels were dried at 40°C until a constant mass was reached. Preparation scheme is presented in Figure 2.

### 3.2. Clay/polymer nanocomposite hydrogel structure

Wide angle (WAXS) or small angle X-ray scattering (SAXS) are generally used methods for characterization of nanocomposite structure. These techniques enable determination of the spaces between structural layers of the silicate utilizing Bragg’s law: sinθ=nλ/2d, where λ corresponds to the wave length of the X-ray radiation used in the diffraction experiment, d the spacing between diffraction lattice planes and θ is the measured diffraction angle [70]. By monitoring the position, shape and intensity of the basal reflection from the distributed silicate layers, the nanocomposite structure may be identified [71].

Depending on the nature of the components used (clay mineral, organic cation and polymer matrix) and the method of preparation, three main types of composites may be obtained when a clay mineral is combined with polymer. Then the polymer is unable to be intercalated, a phase-separated composite is obtained, whose property stay in the same range as those of traditional micro composites. Beyond this classical family composite, two further types of nanocomposites can be obtained. An intercalated structure in which a single (and sometimes more than one) extended polymer chain is intercalated between the silicate layers results in well-ordered multilayers morphology built up of alternating polymeric and inorganic layers. When the silicate layers are completely and uniformly dispersed in a continuous polymer matrix, an exfoliated or delaminated structure is obtained [70] Intercalated structures can be identified using SAXS or WAXS analyses [46,72].

To analyse the effect of monomer, crosslinker and photoinitiator content on composite structure formation we have prepared dispersion of MMT particles, monomer, crosslinker and photoiniciator to study the influence of reagents on MMT particles intercalation by measuring distances between silicate galleries of clay particles using small angle X-ray scattering (SAXS). Figure 3 shows two x-ray diffraction curves of O-MMT particles which were dispersed in monomer, crosslinker and photoinitiator water dispersion.

On the diffraction curve of O-MMT particles dispersed in water, the characteristic maximum for O-MMT particles (q= 2,8 nm-1) is observed. According to the Braggs law it corresponds to the distance between silicate layers d001 = 2.03 nm. By the addition of monomer, crosslinker and photoinitiator into the O-MMT dispersion, the characteristic discrete maximum on the diffraction curve is shifted to a lover angle value (q=1,65nm-1) which corresponds to the distance between silicate layers d001 = 3,81 nm-1. According to the pronounced change in silicate layers distances, we are concluding that monomer molecules have intercalated between silicate layers.

Thereby silicate layers are pushed apart which increases the distance between them, however the repetitive silicate multi layer structure is still preserved, allowing the interlayer spacing to be determined. By addition of monomer, crosslinker and photoinitiator into O-MMT aqueous dispersion, we obtained O-MMT dispersion with intercalated structure of O-MMT particles as shown in Figure 4.

Since nanocomposite material is formed when the complete exfoliation of silicate platelets is possible, in-situ polymerized hydrogels were also analyzed using SAXS. Figure 5 presents x-ray spectra of composite hydrogels with different concentrations of O-MMT particles (0,25; 0,5; 0,75; 1 wt%).

The discrete maximum at q=1.65 nm-1 characteristic for O-MMT particles dispersed in monomer solution, disappears on small angle scattering curves of nanocomposite hydrogels. This phenomenon indicates that monomer molecules between platelets galleries polymerize and crosslink due to UV irradiation. Polymer formation causes movement of clay platelets apart and thereby the exfoliated structure of polymerized O-MMT/NIPAM nanocomposite hydrogel is formed.

In contrast to the intercalated structure, the extensive layer separation associated with exfoliated structures disrupts the coherent layer stacking and results in a featureless diffraction patters. Thus, for exfoliated structures no more diffraction peaks are observed in X-ray diffractograms either because of a much too large spacing between the layers, (i.e. exceeding 8 nm in the case of ordered exfoliated structure) or because the nanocomposites did not present ordering [70,71,73].

### 3.3. Clay/polymer nanocomposite hydrogel swelling and gel fraction

The weight ratio of the dried hydrogels in rinsed and unrinsed conditions can be assumed as a measure of crosslinking degree or gel fraction. Therefore the gel fraction of sample can be calculated as follows [74]:

Gel fraction ( % ) = W f W c W i W c 100

Where Wf and Wi are the weight of the dried hydrogel after and before rinsing, respectively and Wc is the weight of organoclay incorporated into the sample.

To perform gel fraction measurement, pre-weighed hydrogel sample was dried under vacuum at room temperature until no change in mass was observed.

A typical dependency of the gel fraction on the clay concentration in hydrogels is given in Figure 7.

Gel fraction of samples is increased by increasing the amount of clay. The relationship is almost linear. The gel fraction data reveal that presence of clay within the three dimensional networks of hydrogels causes an increase in crosslinking, thus creates more entangled structure. By adding O-MMT to the hydrogel, strong interactions are developed between functional groups of organoclay and polymer chains.

When pre-weighed samples of nanocomposite hydrogels are kept in water, the compact (dry) network structure of the polymer matrix relaxed and swells due to the diffusion of water molecules into the matrix until equilibrium is reached. At this stage, pressure inside the hydrogel matrix increases due to the presence of large amount of water molecules. Crosslinked structure prevents the dissolution of hydrogels [43].

For determination of an equilibrium swelling degree (EDS), we used pre-weighted hydrogel samples and immersed them into deionised water. Samples were removed from water every hour, wiped with filter paper in order to remove surface water, weighted and placed back into the water for further swelling. The equilibrium was reached when no mass difference was determined. EDS was calculated using the equation [46]:

E D S ( % ) = W s W d W d 100 E1

where Ws and Wd are the masses of the gel in swollen and dried states, respectively.

When hydrogel is exposed to water, water molecules diffuse into hydrogel structure and consequently hydrogel swells. Hydrogel ability to swell or uptake water is one of its key characteristics.

Figure 8 demonstrates the equilibrium degree of swelling (EDS) of NIPAM hydrogel and NIPAM/clay nanocomposite hydrogels as a function of the amount of clay. Decreasing trend of equilibrium swelling degree by increasing the quantity of organoclay is observed.

By comparing the equilibrium swelling degree and gel fraction values (Figure 7) a relationship between these properties is observed, i.e. more gel fraction leads to less swelling. Denser hydrogel structure which is formed by increasing clay particles concentration affects the water uptake and decreases the swelling degree. Water uptake represents the migration of water molecules into preformed gapes between polymer chains [75]. Denser hydrogel structure diminish the accessibility of water molecules to hydrophilic parts of polymer molecules, therefore less water can penetrate into the hydrogel structure.

### 3.4. Clay/polymer nanocomposite hydrogel morphology

Figure 9 shows SEM micrographs of a cross-section and a pore surface of nanocomposite hydrogels with different clay content. Samples were lyophilized after the equilibrium swelling has been reached at room temperature in order to preserve natural nanocomposite hydrogel structure in swollen state. Nanocomposite hydrogel cross-section (Figure 9 A/I, B/I, C/I, D/I) shows very porous structure with several pores and wide pore size distribution. The pore structure has a sponge-like shape with spherical opens and interconnected cells. This porous microstructure is essential for a large active surface of hydrogel and assures the capillary effect of water uptake. Comparing the hydrogels pore structure regarding the clay content we observed a drastic change in pore size for nanocomposite hydrogel with 1 wt% O-MMT particles in the hydrogel matrix. At the concentration of 0.25 % O-MMT particles the pore size is approximately 200 μm, while the pore size for nanocomposite hydrogel with 1% O-MMT particles is 100 μm. This pore size reduction confirms that silicate platelets represent additional crosslinking points in nanocomposite hydrogel structure.

Figures 9 A/II, B/II; C/II and D/II show pore surfaces of nano-hydrogels. On the surface incorporated clay particles are observed.

## 4. Adsorption properties of clay/polymer nanocomposite hydrogels

Adsorption studies are the key for evaluating the effectiveness of an adsorbent. Montmorillonite particles used for preparation of nanocomposite hydrogels are organically modified and therefore contain positively charged nitrogen atoms that attract opposite negatively charged anions with electrostatic attraction. Binding efficiency was studied with determination of adsorption degree. To study the effects of different experimental parameters, such as, pH, dye concentration, clay structure on the adsorption of anionic dye Acid Orange 33 onto clay/polymer nanocomposite hydrogel, UV spectroscopy was used. A Carry 50 spectrophotometer (Varian) was used for analyses. The dye concentration was determined at a wavelength corresponding to the maximum absorbance. The adsorption degree was calculated using following equation [43]:

Adsorption degree ( % ) = C 0 C e C 0 100

Where C0 and Ce are the initial and equilibrium concentrations of Acid Orange 33 dye (mg/L), respectively.

Acid Orange 33 is an anionic dye used for dyeing wool, silk and PA, since it contains negatively charged SO3 - groups in the structure (Figure 10).

### 4.1. Adsorption degree: pH dependence

pH of the solution is one of the main parameters that control the adsorption process. The effect of pH solution depends on the ions present in the reaction mixture and electrostatic interactions at the adsorption surface [43]. To determine the effect of different pH on Acid Orange 33 dye removal, the adsorption was carried out at different pH values of dye solution (pH= 3-9). pH was adjusted using acid/base buffer solutions. Figure 11 presents the effect of pH on the dye adsorption at an initial dye concentration of 100 mg/L.

In Figure 11 the highest dye adsorption degree is observed at pH = 3 (around 60%). We assume that this high dye adsorption onto clay/polymer nanocomposite hydrogel at low pH values is due to the neutralization of the negative charge of –SO3- anion, which influences the protonation and thereby increases the electrostatic attraction between the negatively charged –SO3- anion and the positively charged adsorption site. The reason for high adsorption capacity at low pH is due to the strong electrostatic interaction between the cationic surfactant head groups of clay minerals incorporated in the hydrogel matrix and dye anions [4].

By increasing the pH to higher, neutral values (pH=4-7) we observe a decrease in adsorption degree. This is due to the decease of positive charge on the clay surface and the number of negatively charged sites increases. The negatively charged surface sites on clay do not favour the adsorption of anionic dye due to the electrostatic repulsion [76].

In alkaline pH region (pH=8-9) we observe another slight increase in adsorption degree, which is lower regarding the adsorption at pH = 3. Barkaralingam et al. reported that in alkaline medium a competition between OH- ions and dye anions will be expected [76], however a significant colour adsorption is still observed as the pH of dye solution increases from 7 to 9. He suggested that a second mechanism is operating at these conditions. The mechanism of colour removal at higher pH values can be explained by formation of covalent bonds between the external surface –OH groups of Si and Al atoms of adsorbent and negatively charged dye molecules [10].

The maximum adsorption degree of Acid Orange 33 is at pH =3, which was therefore selected for all further adsorption experiments.

The effect of adsorption time on the adsorption capacities of Acid Orange 33 is shown in Figure 12. The adsorption capacity increased rapidly within the first 60 minutes, after that it increased slowly until the adsorption equilibrium was reached. Under experimental conditions (1 wt% O-MMT, 0,1g/L Acid Orange 33 and pH3), the equilibrium time for the adsorption of Acid Orange 33 onto clay/polymer nanocomposite is 360 minutes. The rapid adsorption observed during the first 60 minutes is probably due to the abundant availability of active sites on the clay surface, and with the gradual occupancy of these sites, the adsorption becomes less efficient [77].

### 4.3. Adsorption degree - initial dye concentration dependence

Generally, the removal of dye is dependent on the initial concentration of the dye in the solution. Results shown in Figure 13 indicate that the equilibrium dye uptake by nanocomposite hydrogel increases with increasing initial dye concentration. This is because at higher initial dye concentration, the availability of the number of dye molecules is higher, which can easily penetrate through hydrogel matrix. However, the removal efficiency is increasing only slightly after the initial dye concentration 0.05 g/L. This can be due to the saturation of hydrogel sites [43] or due to the fact that the formation of dye molecules agglomerates makes it almost impossible for them to diffuse deeper into the nanocomposite hydrogel [78].

### 4.4. Adsorption degree - O-MMT clay particles concentration dependence

The effect of the amount of active sites was studied by using hydrogels with different concentration (0.25 – 5%) of O-MMT particles incorporated in hydrogel matrix. The adsorption degree was measured in a solution containing 100 mg/L Acid Orange 33 dye at pH3. Figure 14 shows that the removal of the dye from the solution increases with an increase in the quantity of O-MMT particles incorporated into the hydrogel matrix. This indicates that the presence of higher quantity of O-MMT particles provides a larger number of active sites, which are positively charged and are capable to absorb more Acid Orange 33 dye molecules due to electrostatic forces. From the results we can conclude that the adsorption degree is significantly increasing from 30 to 59,9% when the concentration of nanoparticles increases (from 0.25 to 1% of O-MMT), but with additional increase of O-MMT particles in hydrogel matrix there is no change in the adsorption degree (the adsorption degree is 60,3% for the hydrogel containing 5% of O-MMT ). We assume that at higher clay concentrations agglomerates are formed inside the hydrogel matrix, and therefore the expected additional active sites are not formed [78].

## 5. Conclusions

Hydrogel nanocomposites have been prepared and their potential to be used as adsorbent materials for the removal of dyes which is a serious problem, especially in the textile industry was studied.

It was shown that incorporation of O-MMT particles into the hydrogel matrix induced adsorption capability for acid dye Acid Orange 33. The results obtained from absorption study show that:

The adsorption capacity is maximal at the pH value 3 of the dye solution and is decreasing with increasing pH.

The equilibrium time for the adsorption of Acid orange 33 onto clay/polymer nanocomposite is 360 minutes.

Equilibrium dye uptake by nanocomposite hydrogel increases with increasing initial dye concentration.

As the content of O-MMT particles in hydrogel matrix increases, adsorption capacity is increasing. At O-MMT content higher than 1wt% the adsorption capacity remains unchanged.

## References

1. 1. Akar S. T. Uysal R. Untreated clay with high adsorption capacity for effective removal of C.I. Acid Red 88 from aqeous solutions: Batch and dynamic flow mode studies. Chemical Engineering Journal 2010 162 591 598
2. 2. Ojstrsek A. Fakin D. 2011 Colour and TOC reduction using biofilter packed with natural zeolite for the treatment of textile wastewater Desalination and Water Treatment 33 147 155
3. 3. Bennani Karim. A. Mounir B. Hackar M. Bakasse M. Yaacoubi A. Removal of Basic Red 46 dye from aqueous solution by adsorption onto Moroccan clay Journal of Hazardous Materials 2009 168 304 309
4. 4. Özcan A. Ömeroğlu Ç. Erdoğan Y. Özcan A. S. Modification of bentonite with a cationic surfactant: An adsorption study of textile dye vReactive Blue 19 Journal of Hazardous Materals 2007 140 173 179
5. 5. Rafatullah M. Sulaiman O. Hashim R. Ahmad A. Adsorption of methylene blue on low-cost adsorbents: A review Journal of Hazardous Materials 2010 177 70 80
6. 6. Gürses A. Doğar Ç. Yalçin M. Açikyildiz Bayrak R. Karaca S. The adsorption kinetics of the cationic dye, methylene blue, onto clay Journal of Hazardous Materials 2006 B131 217 228
7. 7. Gil A. Assis F. C. C. Albeniz S. Korili S. A. Removal of dyes from wastewaters by adsorption on pillared clays Chemical Engineering Journal 2011 168 1032 1040
8. 8. Lin S. Juang R. Wang Y. Adsorption of acid dye from water onto pristine and acid-activated clays in fixed beds Journal of Hazardous Materials 2004 B113 195 200
9. 9. Li S. Removal of crystal violet from aqueous solution by sorption into semi-interpenetratined networks hydrogels constituted of poly(acrylic acid-acrylamide-methacrylate) and amylose Boiresource Technology 2010 101 2197 2202
10. 10. Baskaralingam P. Pulikesi M. Ramamurthi V. Sivanesan S. Equilibrium studies for the adsorption of Acid dye onto modified hectorite Journal of Hazardous Materials 2006 B136 989 992
11. 11. Namasivayam C. Arasi D. J. S. E. Removal of Congo Red from wastewater by adsorption onto waste red mud Chemosphere 1997 34 2 401 417
12. 12. Namasivayam C. Yamuna R. T. Removal of Congo Red from aqueous solutions by biogas waste slurry Journal of Chemical Technology and Biotechnology 1992 53 22 153 157
13. 13. Namasivayam C. Kanchana N. Waste banana pith as adsorbent for colour removal from wastewaters Chemosphere 1992 25 11 1691 1705
14. 14. Namasivayam C. Muniasamy N. Gayathri K. Rani M. Ranganathan K. Removal of dyes from aqueous solutions by cellulosic waste orange peel Bioresource Technology 1996 57 1 37 43
15. 15. Pavlidou S. Papaspyrides C. D. A review on polymer-layered silicate nanocomposites Progress in polymer science 2008 33 1119 1198
16. 16. Singa Ray S. Okamoto M. 2003 Polymer/layered silicate nanocomposites: a review from preparation to processing Progress in Polymer Science 28 1539 1641
17. 17. Fischer H. 2003 Polymer nanocomposites: from fundamental research to specific applications Material Science and Engineering C23 763 772
18. 18. Zeng Q. H. Yu A. B. Lu G. Q. Paul D. R. 2005 Clay-based polymer nanocomposites: research and commercial development Journal of Nanoscience and Nanotechnology 5 1574 1592
19. 19. Gil A. Gandia L. M. Vicente M. A. Recent advances in the synthesis and catalyticapplications of pillared clays Catalysis Reviews, Science and Engineering 2000 42 145 212
20. 20. De Stefanis A. Toklinson A. A. G. 2006 Towards designing pillared clays for catalysts Catalysis Today 114 126 141
21. 21. Shichi T. Takaqi K. Clay minerals as photochemical reaction fields Journal of Photochemistry and Photobiology C: Photochemistry Reviews 2000 a 113 130
22. 22. Burst J. F. 1991 Application of clay minerals in ceramics Applied Clay Science 5 421 443
23. 23. Bundy W. M. Ishley J. N. Kaolin in paper filling and coating Applied Clay Science 1991 5 397 420
24. 24. Mousty C. Sensors and biosensors based on clay-modified electrodes- new trends Applied Clay Science 2004 27 159 177
25. 25. Liu P. Zhang L. Adsorption of dyes from aqueous solutions of suspensions with clay nano-adsorbents Separation and Purification Technology 2007 58 32 39
26. 26. Meunier A. 2005 Clays. Heidelberg: Springer-Verlag Berlin.
27. 27. Wang L. Wang A. Adsorption properties of Congo Red from aqueous solution onto surfactant-modified montmorillonite Journal of Hazardous materials 2008 160 173 180
28. 28. Betega de Paiva L. Morale A. R. Díaz F. R. V. 2008 Organocalys: Properties, preparation and applications Applied Clay Science 42 8 24
29. 29. Lagaly G. Ziesmer S. Colloid chemistry of clay minerals: the coagulation of montmorillonite dispersions Advances in Colloid and Interface Science 2003 100-102 100 102
30. 30. Gieseking J. E. 1939 The mechanism of cation exchange in the montmorillonite-beidellite-nontronite type of clay minerals Soil Science 47 1 14
31. 31. MacEwan D. M. C. 1944 Identification of the montmorillonite group of minerals by X-rays Nature 154 577 578
32. 32. Theng B. K. G. 1974 The chamistry of Clay-Organic Reactions. London: Adam Hilger.
33. 33. Lagaly G. 1984 Clay-organic interactions Transactions of the Royal Society of London 211 315 332
34. 34. Yariv S. Cross H. 2002 Ograno-Clay Complexes and Interaction. Marcel Dekker.
35. 35. Errais E. Duplay J. Darragi F. M´Rabet I. Aubert A. Huber F. Morvan G. Efficient anionic dye adsorption on natural intreated clay: Kinetic study and thermodynamic parameters Desalination 2011 275 74 81
36. 36. Ojstrsek A. Doliska A. Fakin D. 2008 Analysis of reactive dyestuffs and their hydrolysis by capillary electrophoresis Analytical Science 24 1581 1587
37. 37. Wang L. Wang A. Adsorption properties of Congo Red from aqueous solution onto surfactant-modified montmorillonite Journal of Hazardous Materials 2008 160 173 180
38. 38. Koswojo R. Utomo R. P. Ju Y. Ayucitra A. Soetaredjo F. E. Sunarso J. Ismadji S. 2010 Acid Green 25 removal from wastewater by organo-bentonite from Pacitan Applied clay science 48 81 86
39. 39. Ceyhan Ö. Baybas D. Adsorption of some textile dyes by hexadecyltrimethylammonium bentonite Turkish Journal of Chemistry 2001 25 193 200
40. 40. Zohra B. Aicha K. Fatima S. Nourredine B. Zoubir D. Adsorption of Direct Red 2 on bentonite modified by cetyltrimethylammonium bromide Chemical Engineering Journal 2008 136 295 305
41. 41. Liu B. Wang X. Yang B. Sun R. Rapid Modification of montmorillonite with novel cationc Gemini surfactants and its adsorption for methyl orange Materials Chemistry and Physics 2011 130 1220 1226
42. 42. Yang Y. Q. Han S. Y. Fan Q. Q. Uqbolue S. C. 2005 Nanoclay and modified nanoclay as sorbents for anionic, cationic and nonionic dyes Textile research journal 75 622 6
43. 43. Taleb M. F. A. Hegazy D. E. Ismail S. A. Radiation synthesis characterization and dye adsorption of alginate-organophilic montmorillonite nanocomposite Carbohydrate Polymers 2012 87 2263 2269
44. 44. Shirsath S. R. Hage A. P. Zhou M. Sonawane S. H. Ashokkumar M. Ultrasound assisted preparation of nanoclay Bentonite-FeCo nanocomposite hybtrid hydrogel: A potential responsive sorbent for removal of organic pollutant from water Desalination 2011 281 429 437
45. 45. Dalaran M. Emik S. Güçlü G. İyim T. B. Özgümüş S. Study on a novel polyampholyte nanocomposite seperabsorbent hydrogels: Synthesis, characterization and investigation of removal of indigo carmine from aqueous solution Desalination 2011 297 170 182
46. 46. Li S. Zhang H. Feng J. Xu R. Liu X. Facile preparation of poly(acrylic acid-acrylamide) hydrogels by frontal polymerization and their use in removal of cationic dyes from aqueous solution Desalination 2011 280 95 102
47. 47. Janovak L. Varga J. Kemeny L. Dekany I. Swelling properties of copolymer hydrogels in the presence of montmorillonite and alkylammonium montmorillonite Applied clay science 2009 42 260 270
48. 48. Osada Y. 2001 (editor). Gels Handbook. San Diego: Academic Press.
49. 49. Ramírez E. Burillo S. G. Barrera-Díaz Roa G. Bilyeu B. Use of pH-sensitive polymer hydrogels in lead removal from aqueous solution Journal of Hazardous Materials 2011 192 432 439
50. 50. Haraguchi K. 2007 Nanocomposite hydrogels Current Opinion in Solid State and Materials Science 11 47 54
51. 51. Haraguchi K. 2007 Nanocomposite Gels: New Advanced Functional Soft Materials Macromolecular Symphosium 256 120 130
52. 52. Nguyen K. T. West J. L. Photopolymerizable hydrogels for tissue engineering applications Biomaterials 2001 23 4307 4314
53. 53. Bulut Y. Akcay G. Elma D. Serhatli I. E. Synthesis of clay-based superabsorbent composite and its sorption capability Journal of Hazardous Matererials 2009 171 717 723
54. 54. Haraguchi K. Li H. J. Mechanical properties and structure of polymer-clay nanocomposite gels with high clay content Macromolecules 2006 39 1898 1905
55. 55. Kaplan M. Kasgoz H. Hydrogels nanocomposite sorbents for removal of basic dyes Polymer Bulletin 2011 67 1153 1168
56. 56. Xia X. H. Yih J. DSouza N. A. Hu Z. B. Swelling and mechanical behavior of poly(N-isopropylacrylamide)/Na-montmorilonite layered silicates composite gels Polymer 2003 44 3389 3393
57. 57. Zhou S. H. Yang J. G. Wu C. P. 2003 Synthesis and swelling properties of poly (N,N`-diethylacrylamide)-clay nanocomposites Acta Polymer Sinica 3 326 329
58. 58. Bignoti F. Satore L. Penco M. Ramorino G. Peroni I. Effect of montmorillonite on the properties of thermosensitive poly(N-isopropylacrylamide) composite hydrogels Journal of Applied Polymer Science 2004 93 1964 1971
59. 59. Xiang Y. Q. Peng Z. Q. Chen D. J. 2006 A new polymer/clay nano-composite hydrogel with imporved response rate and tensile mechanical properties European Polymer Journal 42 2125 2132
60. 60. Liang L. Liu J. Gong X. Thermosensitive poly(N-isopropylacrylamide)-clay nanocomposites with enhanced temperature response Langmuir 2000 16 9895 9899
61. 61. Xu K. Wang J. H. Xiang S. Chen Q. Zhang W. D. Wang P. X. Study on the synthesis and performance of hydrogels with ionic monomers and montmorillonite Applied Clay Science 2007 38 139 145
62. 62. Zhang Q. Li X. Zhao Y. Chen L. Preparation and performance of nanocomposite hydrogels based on different clay Applied Clay Science 2009 46 346 350
63. 63. Nie J. J. Du B. Y. Oppermann W. 2005 Swelling, elasticity and spatial inhomogeneity of poly(N-isopropylacrylamide)/clay nanocomposite hydrogels Macromolecules 38 5729 5736
64. 64. Yi J. Ma Y. Zhang L. Synthesis and decoloring properties of sodium humate/poly (N-isopropylacrylamide) hydrogels Bioresource Technology 2008 99 13 5362 5367
65. 65. Kasgöz H. Durmus A. Dye removal by a novel hydrogel-clay nanocomposite with enhanced swelling properties Polymers for Advanced Technologies 2008 19 838 845
66. 66. Nguyen K. T. West L. J. Photopolymerizable hydrogels for tissue engineering applications. Biomaterials 2002 23 4307 4314
67. 67. He D. Susanto H. Ulbricht M. 2009 Photo-irradiation for preparation, modification and stimulation of polymeric membranes Progress in Polymer Science 34 62 98
68. 68. Tamirisa P. A. Koskinen J. Hess D. W. Plasma polymerized hydrogel thin films Thin Solid Films 2006 515 2618 2624
69. 69. Hongyan H. Ling L. James Lee. L. Photopolymerization and structure formation of methacrylic acid based hydrogels in water/ethanol mixture Polymer 2006 47 1612 1619
70. 70. Kurecic M. Sfiligoj-Smole M. Stana-Kleinschek K. 2012 UV polymerization of poly(N-isopropylacriylamide) hydrogel Materials and technology 46 69 73
71. 71. Alexandre M. Dubois P. 2000 Polymer-layered silicate nanocomposites: preparation, properties and uses of a new class of materials Materials science and engineering:R:Reports 28 1 63
72. 72. Pavlidov S. Papaspyrides C. D. 2008 A review on polymer-layered silicate nanocomposites Progress in Polymer science 33 1119 1198
73. 73. Haraguchi K. Li H. J. Mechanical properties and structure of polymer-clay nanocom- poiste gels with high clay content Macromolecules 2006 39 1898 1905
74. 74. Vaia R. A. Giannelis E. P. Polymer melt intercalation in organicallymodified layered silicates: model predictions and experiment Macromolecules 1997 30 8000 9
75. 75. Kokabi M. Sirousazar M. Hassan Z. M. PVA-clay nanocomposite hydrogel for wound dressing European Polymer Journal 2007 43 773 781
76. 76. Can V. Abdurrahmanoglu S. Okay O. Unusual swelling behavior of polymer-clay nanocomposite hydrogels Polymer 2007 48 5016 5023
77. 77. Baskaralingam P. Pulikesi M. Elango D. Ramamurthi V. Sivanesan S. Adsorption of acid dye onto organobentonite Journal of Hazardous Materials 2006 B128 138 144
78. 78. Errais E. Duplay J. Darragi F. M´Rabet I. Aubert A. Huber F. Morvan G. Efficient anionic dye adsorption of natural intreated clay:Kinetic study and thermodynamic parameters Desalination 2011 275 74 81
79. 79. Kurecic M. 2011 Synthesis of ion exchange nanocomposite hydrogels inside the PP membrane pores. PhD thesis.

Written By

Manja Kurecic and Majda Sfiligoj Smole

Submitted: February 29th, 2012 Published: September 27th, 2012